Porter Easter Ling Solutions
Short Description
kinetics...
Description
Solutions to Exercises Compiled by lohn C. Ion
Chapter 1 1.1
Cp
= 22.64 + 6.28
x 1O 3 T J mol1K 1
Entropy increase, flS flS3001358
=
=
f
T 2C
TI
f
1358
22.64
+ 6.28 x 1O 3 T
300
=
2dT T T
l~öll[22.641n T
dT
+ 6.28 x 1O 3 Tj
= 40.83 J mol1K 1 1.2
Liquid Fe
,
_  
1600 y·Fe
~
::::l
~ ~ E {E.
800 500
_______
~_c
aFe
300
o
50
100 Pressure, kbar
150
442
Solutions 10 exercises Liquid Fe
aFe
'Y Fe
yFe
At 1600"C
>L
24
At 800"C
22
",e> ",,,,
u:'"
(I)
Pressure kbar
o.Fe yFe
tFe
120
110 Schematic free energypressure curves for pure Fe.
1.3
From Equation 1.14
(~~)eq 
::v
Assuming !1H and !1 V are independent of T and P for the range of interest, the equation may be rewritten as
where: !1H !1V T
= HL
H S = 13050 J molI; = V L  V S = (8.0  7.6) x 1O 6m3 ; = (1085 + 273) K. 
Thus if !1P is 10 kbar, i.e. 109 Nm 2 , the change in the equilibrium melting temperature is given by the above equation as !1T
= 42 K
Solutions to exercises 1.4
443
Phases stable at low temperatures must have low enthalpies because the ( TS) term in the expression for G becomes negligible. Phases stable at high temperatures, on the other hand, have higher entropies to compensate for higher enthalpies.
1.5
Six distinguishable configurations.
Theoretical number of distinguishable ways of arranging two black balls and two white balls in a square is
(NB + N w )! NB! N w ! 1.6
=
(2 + 2)! 2! 2!
=
6 
Dividing both sides of Equation 1.30 by the number of moles of solution (nA + nB) gives dG'
    = JlA
(nA + nB)
dnA dnB + JlB ,=(nA + nB) (nA + nB)
The lefthand side of this equation is the free energy change per mole of solution and can therefore be written dG.
dnA ...:...:...,an d (nA + nB)
dnB (nA + nB)
are the changes in the mole fractions of A and B, dXA and dXB . The above equation can therefore be written as
444
Solutions to exercises
+ IlB dXB
dG = IlA dXA
dG dXA Thus dXB = IlA dXB = IlA
+ IlB
+ IlB
(1.6.1)
But using Equation 1.31
G = Il A X A
+ IlB X B
. G  Il A X A glves IlB = XB .. dG glvmg dXB = IlA
+
G  Il A X A XB
dG or IlA = G  X B dXB From the figure IlA
= PR
 X B (QR) XB
= PQ = OS
i.e. point S, the extrapolation of the tangent to point R on the Gcurve represents the quantity IlA. Equation 1.6.1 gives IlB =
dG
+ dXB
IlA

i.e. IlB = OS
UV
+ US
But US = OT = 1 Thus IlB = OS + UV = TV i.e. point V represents the quantity IlB.
>
v
~
Cl)
c:
Cl) Cl) Cl)
u:
I I
tGL 
s
u
I
o __~I~peT A
B
Solutions to exercises 1.7
Equation 1.31: G = IlAXA + IlBXB Equation 1.39: G = XAG A + XBG B + OXAXB + RT(XAlnXA + XBlnXB) = XAG A + XBG B + Q(XiXB + X~XA) + RT(XAlnXA + XBlnXB) = XA[G A + QX~ + RTlnXA] + XB[G B + oxi + RTlnXB] Comparison with Equation 1.31 and using X A IlA = GA IlB =
1.S
445
GB
+ XB
=
1 gives
+ Q(1  X A)2 + RTlnXA
+ Q(1
 X B)2
+ RTlnXB
(a) Atomic weight of Au = 197 Atomic weight of Ag = lOS 15 No. of moles of Au = 197 = 0.076 25 No. of moles of Ag = lOS = 0.231 no. of moles of solution = 0.307 . 0.076 (b ) Mole fractiOn of Au = 0.307 = 0.24S . 0.231 Mole fractiOn of Ag = 0.307 = 0.752 (c) Molar entropy of mixing, ASmix AS mix
=
R(XAlnXA + XBlnXB)
= S.314(0.24S·lnO.24S + 0.752· In 0.752) =
4.66 J K 1 mol 1
(d) Total entropy of mixing = Molar entropy of mixing x no. of moles of solution = 4.66 x 0.307 = 1.43 J K 1 (e) Molar free energy change at 500°C = AG mix = RT(XAlnXA + XBlnXB) .. AG mix = TASmix = 773 x 4.66 = 3.60 kJ mol 1 (f) IlAu = GAu + RTlnXAu = 0 + (S.314· 773 ·ln 0.24S) = S.96kJ mol 1
Solutions to exercises
446
GAg + RTlnXAg 0 + (8.314·773· In 0.752) = 1.83 kJ molI
=
IlAg
=
(g) For a very small addition of Au dG'
=
IlAu· dnAu(T, P, nB constant)
At 500°C, IlAu
= 8.96 kJ
molI.
Avogadro's Number = 6.023
1 eV = 1.6
X
X
1023
10 19 J
8.96 kJ mol
I
=
1.6
8.96 X 1019 X
= 0.1
103 6.023
X
X 1023
eVatom
I
eVatom 1
. . Adding one atom of Au changes the free energy of solution by 0.1 eV.
1.9
~\~r 1.9
a
t
CD
c: Q)
Q)
Q)
Graphite T
_ c
>Cl
u:
8
e
b
d
= T,
447
Solutions to exercises
n
0
h
i c
d   Fe 3 C   Graphite
Graphite
Fe
%C.
Gcomposition and Tcomposition diagrams tor the FeFe3C and FeC systems (not to scale).
1.10
dCu
= Ill dnA
dCß = +Il~ dnA
At equilibrium dCu + dCß = 0 i.e. Ill dnA + Il~ dnA = 0 i.e. III = Il~ Similarly for B, C, etc. 1.11
Equilibrium vacancy concentration e
Xv
=
I1Cv
exp  RT I1S
I1H
R
RT
v v = exp ·exp 
1 eV = 1.6 X 10 19 J .. R = 8.63 X 10 5 eV atom 1 K 1 X~ (933 K) = exp (2) . exp ( 8.63 =
3.58
X
2.28
X
0.8 10 5
933
X
10 4
X~ (298 K) = exp (2) . exp ( 8.63 =
X
10 13
X
0.8 10 5
X
298
)
)
Solutions to exercises
448 1.12
Assurne X Si
= A exp 
Q RT
Q
InXsi = InA  RT
At 550°C (823 K): In 1.25 = InA  Q/(8.314 x 823) At 450°C (723 K): In 0.46 = InA  Q/(8.314 x 723) which can be solved to give Q = 49.45 kJ mol 1 A = 1721 Thus at 200°C (473 K) 49450 ) X Si = 1721· exp  ( 8.314 x 473
= 0.006 atomic % According to the phase diagram, the solubility should be slightly under 0.01 atomic %. Reliable data is not available at such low temperatures due to the long times required to reach equilibrium. 1.13
A sketch of the relevant phase diagram and free energy curves is helpful in solving this problem. See p. 449. I1G A and 11GB are as defined in (b) and (c).
Since A and Bare mutually immiscible, the tangent to the liquid curve G L at X B = X~ will intercept the curves for the A and B phases as shown, i.e. IlÄ = G1, Il~ = G~. The liquid is assumed ideal, therefore from Fig. 1.12 I1G A
= RTElnXÄ
11GB
=
and RTElnX~
But I1G A and 11GB can also be found from the relationships shown in Figs (b) and (c). If C~
=
C~, Equation 1.17 gives
L I1G=·I1T Tm
or
Solutions to exercises
I~ (b)
G~
    TE f"'''''...1 (a)
G~
A
Free energy 01 pure A
t
>.
!:l
Q)
c: Q)
B
6G:G'l
Q)
~
LI..
G~ (d)
xg
A (a) (b) (c) (d)
B
Schematic phase diagram; G T curves for pure A; G T curves for pure B; Free energy curves for the AB system at TE.
Thus 11GA = l1Sm(A)' (Tm(A)  TE) 11GB = l1Sm(B)·(Tm(B)  TE) Finally therefore: RTEInXÄ = l1Sm(A)· (Tm(A)  Td RTEInX~
= l1S m(B)· (Tm(B)
 TE)
or
= 8.4 (1500  TE) 8.314 TEIn (1  XÄ) = 8.4 (1300  TE) 8.314 TEInXÄ
Solving these equations numerically gives
XÄ
449
= 0.44
X~ = 0.56
TE = 826 K
Free energy 01 pure B
450
1.14
So/utions to exercises If solid exists as a sphere of radius r within a liquid, then its free
energy is increased by an amount
G~  G~
= 2yVm
r
(from Equation 1.58)
where G~ is the molar free energy of the sphere and G~ is the molar free energy in the absence of interfaces. Growth of the sphere must lead to a reduction of the total free energy of the system, i.e. growth can occur when G~< GL m . GL  GS >2yV I.e. 00
r
See figure below.
Growth occurs spontaneously with a decrease in free energy
Substituting Equation 1.17 for G L
.
1. e.

G~
AT > '......:..:.:.~ 2yVm Tm rL
Li
Substituting the numerical values given dT(r
AT(r
1.15
=
> 0.2 K nm) > 200 K
1 Ilm)
= 1
Composition = 40% a = 80% ß = 10% y = 10%
A, A, A, A,
20% 5% 70% 20%
B, B, B, B,
40% 15% 20% 70%
C; C; C; C.
gives
Solutions to exercises
Let the mole fractions of a, X ß and y respectively.
x.
451
ß and Y in the final microstructure be X a ,
Balance on A: 0.4 = 0.8 X a + 0.1 X ß + 0.1 X y Balance on B: 0.2 = 0.05 X a + 0.7 X ß + 0.2 X y Balance on C: 0.4 = 0.15 X a + 0.2 X ß + 0.7 X y Solving these equations gives: X a = 0.43; X ß = 0.13; X y = 0.44 1.16 From Equations 1.41 and 1.43 we have
IlA = GA
+ RTlnyAXA
where GA is the free energy of pure A at temperature T and pressure
P.
Suppose GA is known for a given temperature and press ure To and Po i.e. GA(To, Po)
= G?.
From Equation 1.9 for 1 mole of A dGA
= SAdT + VmdP
Thus if SA and Vm are independent of T and P, changing temperature from To to T and pressure from Po to P will cause a total change in GA of
t':1GA = SA(T  To) + Vm(P  Po) GA = G?. + t':1G = G?. + SA(To  T) + Vm(P  Po) and
IlA
= G?. + SA(To 
T) + Vm(P  Po) + RTlnyAXA
The accuracy of this equation decreases as (T  To) and (P  Po) increase.
Solutions to exercises
452 Chapter 2
2.1
(a) Decarburizing gas
Sheet
Carburizing gas
1.4
0.15
L
Carbon concentration
Thickness
(b) Under steadystate conditions, flux of carbon atoms into one side = flux out of the other side = J.
I = _ DcdC dx
{~} = D {~} = D = 2.5 x 1O=~: = 0.32 { dC} j{dC} dx dx D1. 7.7 x 10 D1.4
O. 15
1.4
1.4
0.15
0.15
O. 15 4
(c) Assume that the diffusion coefficient varies linearly with carbon concentration D = a
+ bC
where a and bare constants that can be determined from the data given. Fick's first law then gives
I or
= (a + bC)
f ldx =  f
i.e. lx
dC dx
(a + bC)
dC
bC2
= aC +  2 + d
where dis an integration constant. If we define C
d = aCl

2b Cl2
= Cl at x = 0
Solutions to exercises
453
Similarly, if C = C2 at x = I, the thickness of the sheet, gives b
2
li = aC2 + 2" C2 i.e. 1
=
{a( CI 
aC I

b
2
2" CI

~ (Ci  C~)} /
C2 ) +
I.
The constants a and b can be determined from Dl D2
from
an
= a + bC l = a + bC2
.
WhlCh
a
= D2
(D D l 

2)
C2
Cl  C2
d b  D I  D2  CI  C2
Substitution of these express ions into the equation for 1 gives after simplification
1
= (D2 + DI)CI 2
= 7.7 D2 = 2.5
Substituting: D l
CI
= 1.4 0.8
I C X
X
2
10 11 m 2 s 1 10 11 m 2 s 1
x 60 kg m
3
0.15 3 C2 =   x 60 kg m0.8 = 2 x 10 3 m gives
2.2
1
= 2.4
X
10 6 kg m 2
S1
2
d __
Consider two adjacent (111) planes in an f.c.c. crystal. A vacancy in plane 1 can jump to one of three sites in plane 2. For the sake of
Solutions to exercises
454
generality, let this number of jumps be designated P (=3)0 In all there are 12 possible sites (nearest neighbours)o If nl and n2 are the numbers of vacancies m 2 in planes 1 and 2 respectively, the number of jumps from 1 to 2 will be given by P J y = 12
where
2 m SI
rvnl
r v is the jump frequency of the vacancieso
Likewise
Therefore following the same arguments as in Section 20201 (po 6) gives p 2 ) öCy J y =  ( 12 d r v öx
where dis the perpendicular separation of the adjacent planes, ioeo we can write
In fococo metals the jump distance a is given by
where a is the lattice parameter. For (111) planes d =
;3
Putting P Dy =
=
~~
a
= 3 gives
61 a 2r
y
For (100) planes, adjacent planes are in fact (200)
Solutions to exercises 2.3
455
The activity along the bar is described by the following equation . . achvlty
Ao (x = ·exp  ) 2
4Dt
2~rrDt
where A o = initial activity; D = diffusion constant; t = time;
x
= distance
along the bar.
Thus by plotting In (activity) vs x 2 , a straight line of slope  (4Dt)1 is produced, enabling D to be found since t is known.
x Ilm x2 Il m2
10
20
30
100
400
900
activity
83.8 66.4
42.0
23.6
8.74
In (activity)
4.43
3.74
3.16
2.17
•
4.20
40
50
1600 2500
•
4
• ~
•
.
I.)
c:
m
in
o
ß a
t
b Bulk composition
(ii)
t CI>
I.)
c:: .!!l UJ
Cl
0
a
Xe 
2.9 a t= 0
A
t
ec: m
in
o
xe .....
B
a
t    \1 ß
I I
I I
0.9
t> 0
Solutions to exercises
463
: I
la I I
L
j  I Iß
I I
A
Bulk
0.5

0.9
B
The total distance the interface moves, s, can be calculated in terms of the total couple thickness, L, by writing down an equation describing the conservation of B, i.e. 0.9
(~ + s) + 0 (~  s) =
±
=
0.5L
5.6 x 10 2
Chapter 3 3.1
Considering only nearest neighbours, if a surface atom has B 'broken' bonds, it will have an excess energy of B. E/2, where E is the bond energy. For f.c.c. crystals, each atom has twelve nearest neighbours in the bulk, so that E = L s /6Na , where L s is the molar latent heat of sublimation and Na Avogadro's number (no. of atoms per mole). The surface energy per surface atom is therefore given by Y~v
B Ls 12 Na
= . 
per surface atom
If each surface atom is associated with a surface area A, the surface energy is . B Ls Y =   .  per umt area sv 12A Na
A can be calculated in terms of the lattice parameter a:
464
Solutions to exercises
* Each surface atom is connected to two nearest neighbours in the {220} plane. Therefore it must be connected to ten others out of the plane. Since the atoms are symmetrically disposed about the {220} {hkl}
{200}
{111 }
~~2 ~ a
{220}
~a
A*
a a Y3 Y2'Y2'2
a2
aaY2 ·
B
3
4
5*
Ysv
0.25 [~s]
0.33[;J
Ysv
0.58[a;~J
0.67[a;~J
a
2
2
0.42 [~s
a
]
0.59 [a!;z,J
plane, there must be five bonds above the plane of the paper and five below (giving a total of 12). +It can be shown that in general for f.c.c. met als
+ k 2 + F) 4
a2~(h2
A=~~':'"
For the simple cases above, however, A can be calculated directly from a sketch, as shown.
3.2
E sv = (cos
e + sin 1(1). 2:2
i.e. E sv = (cos 8 + sin 8)';' 2a
dEsv
~
=
(
.
SIll
8
(d!v)e=o = 2:
+ COS 8) . 2aE 2 2
8>0
465
SoLutions to exercises
and E sv = (cos 9  sin 9)· 2:2 ' . h' WhlC glVes At 9
3.3
(dE da
sv )
= 0 there
9=0
9
.. r  1. 96
2r X
106
Thus the smallest diameter
=
1.0 11m
3.7
From the phase diagrams, the limit of solid solubility of Fe in Al is 0.04 wt% Fe, whereas that of Mg in Al is 17.4 wt% Mg. If one element is able to dissolve another only to a sm all degree, the extent of grain boundary enrichment will be large. (See for example Fig. 3.28, p. 138.) Thus grain boundary enrichment of Fe in dilute AlFe alloys would be expected to be greater than that of Mg in AI Mg alloys.
3.8
See Fig. 3.35, p. 145. If da < d ß, then in general the dislocation spacing (D) will span n atom planes in the ß phase and (n + 1) planes in the a phase, i.e.
D = ndß = (n
+
1) da
From the definition of 0 we have
( ve)
Substitution into the first equation gives
n(l i.e. n = and D
=
+ 0) 1
Ö d ~
o
da = (n
+ 1)
da
Solutions to exercises
468
3.9
_   2 x2  __
The edges of the plate exert a force on the periphery of the broad face equal to Y2 . 4· 2.x 2 This force acts over an area equal to (2.x 2)2 IlP = Y2' 4 . ~2 = 2Y2 (2.x 2) X2
The periphery of each edge is acted on by a force of magnitude 2·Y2·2.x 1 + 2·YI·2.x 2 The area of each edge is 2.x I . 2x 2 IlP = 2Y2' 2.x 1 + 2YI ·2.x2 = Y2 2.x 1 ·2x2 X2
+ .2'.!. Xl
From the Wulff theorem (p. 115) for an equilibrium plate shape: XI
YI Y2
=
X2
IlP
(see also Exercise 3.3)
= 2YI = 2Y2 XI
X2
3.10
See Section 3.4.1 (p: 143).
3.11
Atomic radius of Al Atomic radius of Fe
1.43 A = 1.26 A
=
469
Solutions to exercises Hence zone misfit =
=
1.26  1.43 1.43 x 100% 11.89%.
When the misfit is less than 5%, strain energy effects are less important than interfacial energy effects and spherical zones minimize the total free energy. However, when the misfit is greater than 5%, the small increase in interfacial energy caused by choosing a disc shape is more than compensated by the reduction in coherency strain energy. Thus the zones in AlFe alloys would be expected to be discshaped. 3.12
Assuming that the matrix is elastically isotropie, that both Al and Mg atoms have equal elastie moduli, and taking a value of 1/3 for Poisson's ratio, the total elastic strain energy I1G s is given by:
= shear modulus of matrix; o = unconstrained misfit;
Il
V = volume of an Al atom.
o = 1.60 
1.43 = 0.119 1.43 V = 4/3· 1t. (1.43 X 10 10)3 = 1.225 X 10 29 m3 IlAI = 25 GPa = 25 x 109 Nm 2 .. I1Gs = 4 x 25 X 109 x (0.119)2 x 1.225 X 10 29 J atom 1 = 1.735 X 10 20 J atom 1 In 1 mol there are 6.023 I1Gs
= =
1 eV I1G s
= =
1.735
X
X
1023 atoms
10 20 x 6.023 1000
X
1023
kJ mol
1
10.5 kJ mol 1 1.6
X
10 19 J, thus
1 1.735 x 10 20 1.6 x 1019 eVatom
= 0.1 eV atom 1
It is also implicitly assumed that individual Mg atoms are separated by large distances, so that each atom can be considered in isolation, Le. dilute solutions. The use of Equation 3.39 is also based on the assumption that the matrix surrounding a single atom is a continuum.
3.13
See Section 3.4.4. (p. 160).
470
Solutions to exercises
3.14 When a Shockley partial dislocation passes through an f.c.c. crystal the atoms above the glide plane in positions Aare shifted to B positions, B into C positions, etc. i.e. A ~ B ~ C ~ A
A
B
C
A
B L
L
A
L
C
A
B
C
B
B
B
A
A
A
C
B
C
C
C
C
C
B
B
B
B
B
A
A
A
A
A
C
C
C
C
c
e
B
B
B
B
Twin Plane
The above se ries of diagrams shows the twinning process. 3.15 v
•
t
D
~IL_ _   F
Let the interface CD move with a velocity v perpendicular to the interface. Consider unit area of interface perpendicular to both BC and CD. Mass flow perpendicular to BC = u x h. Mass flow perpendicular to CD = v x I. From the conservation of mass: u x h = v x I. u xh I
v=
471
Solutions to exercises
3.16
8
8
8
8
8
8
C
C
C
C
C
C
A
A
A
A
A
A
8
8
8
8
C  C
C 
cI
c
8
8
8
8
8
8
A
A
A
A
A
A
C
C
C
C
C
C
8
8
8
8
8
8
A
A
A
A
A
A
11/11/11/
8
A
I
Fee I
I
I
c
Fee 11
If a single atom in crystal I attempts to jump into a crystal 11 position a ring of dislocation and an unstable A upon A situation results. A Shockley partial dislocation in every {111} slip plane creates a glissile interface between two twinned crystals:
A .1
 
8
A
  ' I               
c
I
..1.
1

_c_________.&.1.... __ '1_ _ _ _ _ _ _ _ _ _8_ I
_A_ _ _ _ _ _ _ _ _ _~...
8
_ ,rAI
.L.
11
c ,..,
_c_________________.1.I.... ___I  8A
I
.1.
A
Note, however, that as a result of the shape change produced by the transformation large coherency stresses will be associated with the interface (see Fig. 3.62a). Similar coherency stresses will arise as a result of the f.c.c./h.c. p. interface in Fig. 3.61. Strictly speaking, Fig. 3.60 is an incorrect representation of the stacking sequence that results from the passage of the partial dislocations. In layer 10, for example, there will not be a sudden change across the 'extra halfplane' of A to B or B to C, but
Solutions to exercises
472
rather a gradual change associated with long range strain fields in both crystals. 3.17 Solid/vapour interfaces and solidIliquid interfaces in nonmetals are faceted and therefore migrate by ledge mechanisms. SolidIliquid interfaces in metals are diffuse and migration occurs by random atom jumps. 3.18 See Section 3.3.4, p. 130. 3.19
From equations 1.41 and 1.43 we can write Ilk
= G B + RT In YiXi
Il~
= GB + RT In YeXe
..
L\1l~
= Il~
YiXi YeXe
= RT I n  
 Il~
For ideal solutions: Yi = Ye = 1 For dilute solutions (Xi « 1): Yi such that in both cases .
L\1l~
Xi
= RT In X
e
This can also be written L\llh = RTln
(1 + Xi~eXe)
If the supersaturation is smalI, i.e.
(Xi  Xe)
«
Xe, then
L\llh = RT (Xi
~eXe)
=
Ye
= constant
(Henry's Law)
473
Solutions to exercises
3.20
a
ß I
T,
 1       
     
I
x~
Suppose the alloy had reached equilibrium at a temperature Tl and consists of long platelike precipitates. The bulk alloy composition is X o, the equilibrium concentrations at Tl and T2 are Xl and X 2 respectively, where T2 is the temperature to which the alloy is heated.
(ii) Interface control
(i) Diffusion control
a_J 1a t~ t,
:L t_~~~_
xß ~
~
x, ____
______
p
~~~~~ x, 
Distance 1 = 12
>
I,
t
_ _ _ _ _ __
[~
t~ t,
_ ~ __   
J
x, 
        
x,             1=
xo            
474
Solutions to exercises
(iii) Mixed control: similar to diffusion control except the interface concentration in the amatrix will be less than X 2 , the equilibrium concentration at T2 • Chapter 4
4.1 Differentiating this equation with respect to r: ddGr
~ =
2
41tr . dGv
+ 81trySL
At the critical radius, r*, this expression is equal to zero
°
41tr*2. dG v + 81tr*YsL
=
r* =2YSL dGv
In order to calculate the critical value of dG, dG * at this radius, the value of r* is substituted into the original equation
YsL dG * = 41t 3 (2dGv )
3
• dG
v
YsL) 2 + 41t (2dG YSL v
161tY~L 3(dGv )2
4.2
From Equation 4.10, at the equilibrium melting temperature Tm
r
n = noexp
(~~~r)
At the equilibrium melting temperature dG v = 0, so that Equation 4.4 be comes
dGr(T = Tm) = 41tr 2YSL For a cluster containing n e atoms with an atomic volume n we have 41t? _ 3 
r.
neU
Therefore the expression for dG r becomes dG r
_41t (3nn )2/3' Y 41t e

475
Solutions to exercises
Substituting n = 1.6 x 1029 m3 and y = 0.177 Jm 2 gives f..G r = (5.435 x 10 20 ) n~/3 For 1 mm 3 , no = 6.25 X 1019 atoms Therefore when n c = 10 atoms, n r = 9 x 1013 clusters mm 3 ; and when nc = 60 atoms, n r = 3 clusters mm 3 ; when nc = 100 atoms, n r = 4 x 10 8 clusters mm 3 ; or, alternatively, 1 cluster in 2.5 x 107 mm 3 (251). 4.3
As the undercooling (f..T) is increased, there is an increasing contribution from f..G y in the equation
whereas the interfacial energy is independent of f..T. Consequently, for a given r, f..G r decreases with increasing f..T, and the 'maximum' cluster size increases somewhat. 4.4
From Equation 4.13 N hom = foCoexp {
16nY~LT~ 3L;kT
1}
. f..T2
where T = Tm  f..T From which the following values are obtained: N hom m 3
f..T K
Sl
7 x 10 7
0.7 8 X 106 1 x 10 12
180 200 220
N hom cm 3 Sl
8 1
X
106
Note the large change in N over the sm all temperature range (see Fig.4.6). 4.5
f..G* = ~. V*· f..G y
For homogeneous nucleation, it has been shown (see 4.1) that r * =2YSL 
f..G y
Thus for a spherical nucleus V*
4nr *3
=
32ny3
SL
3 = 3(f..Gy P
476
Solutions to exercises
ö'G *
= !. V* . ö'G = 161tY~L 2
3ö'G;
v
This is identical to that derived in 4.1, and so the equation holds for homogeneous nucleation. For heterogeneous nucleation, it can be shown that r * =2YSL 
ö'Gv
The volume of a spherical cap on a flat mould surface is given by V
(2 + cos 8)(1  cos 8)2 = 1tr 3 ~'"'~
3
Thus V*
)3 .(2 + cos 8)(1 
= 1t (2YSL ö'Gv
cos 8)2
3
where 8 is the 'wetting' angle. Substituting into the given equation ö'G*
1 4 Y~L = . V*· ö'G =  1 t  . (2 + cos 8)(1 2 v 3 ö'G;
 cos 8)
2
Writing the normal free energy equation for heterogeneous nucleation in terms of the wetting angle 8 and the cap radius r AG
Li

het 
{_i _
1AG
31tr Li
v
+
4 2 } (2 1tr YSL
+ cos8)(1  COS8)2 4
But from Equations 4.19 and 4.17 we have ö'G *
= 161tY~L. (2 + cos 8)(1 3ö'G;
 cos 8)2
4
which is identical to that obtained using ö'G*
= ~V*ö'Gv
4.6
See Section 4.1.3.
4.7
Consider a coneshaped crevice with semiangle a as shown below:
Solutions to exercises
477
R
\
\
\
I
,
I
\ \
,
\
I
I
_
Size of homogeneous nucleus at same /:;.T (same ,")
I
,
" ..... ...... 

",
/
I
I
."
The wetting angle between nuc1eus and mould wall (8) is fixed by the balance of surface tension forces (Equation 4.14). The activation energy barrier (~Gtiet) depends on the shape of the nuc1eus as determined by the angles a and 8. From Equation 4.23, for a given undercooling (~T), ~Gv and r* are constant, such that the following equalities apply
S = ~Gtiet = Vtiet ~Gtiom Vtiom i.e.
S
=
~Gtiet
= Volume of the heterogeneous nucleus
~Gtiom
Volume of a sphere with the same nuc1eus/ liquid interfacial radius
It can be seen that the shape factor (S) will decrease as a decreases, and on cooling below Tm the critical value of ~G * will be reached at progressively lower values of ~T, i.e. nucleation becomes easier. When a ~ 90  8, S = 0 and there is no nuc1eation energy barrier. (It can be seen that a = 90  8 gives a plan ar solid/liquid interface, i.e. r = 00 even for a negligibly small nucleus volume.) Once nuc1eation has occurred, the nuc1eus can grow until it reaches the edge of the conical crevice. However, further growth into the liquid requires the solid/liquid interface radius to pass through a minimum of R (the maximum radius of the cone). This requires an undercooling given by
2YSL = L~T R Tm i.e.
~T= 2YSLTm
RL
478 4.8
Solutions to exercises For conical crevices with a < 90  e the solid/liquid interface can maintain a negative radius of curvature which stabilizes the solid above the equilibrium melting temperature (Tm):
( r)
L
As the temperature is raised above Tm the solid will melt back into the crevice to maintain equilibrium with a radius given by
r=
2YSLTm
LI1T
where (I1T) is now the superheat above Tm· 4.9
If the situation described above is realized in practice it would explain
the observed phenomena. 4.10
(a) The values of the three interfacial energies are as folIows: Solidliquid Liquidvapour Solidvapour
= 0.132 J m 2 ; = 1.128 J m 2 ; = 1.400 J m 2 .
Thus the sum of the solidliquid and liquidvapour interfacial free energies is less than the solidvapour free energy, and there is no increase of free energy in the early stages of melting. Therefore, it would be expected that a thin layer of liquid should form on the surface below the melting point, because the difference in free energies could be used to convert solid into liquid. (b) Imagine the system I below . The free energy of this system is given by:
G(I)
= G S + Ysv
System 11 contains a liquid layer of thickness 0 and solid reduced to a height (1  ö). (The difference in molar volume between liquid and solid has been ignored.)
Solutions to exercises 1 m2
""'....
V
V
S
1m
479
S
L
(1  S)
S 11
Thus G(II) = G S (1  8) + G L 8 + YSL + YLV (8 > 0) G(II) = G S + 8(G L  G S) + YSL + YLV (8) 0) At an undercooling .1T below Tm , G L S L.1T = G + 8 + YSL + Tm L.1T or G(II) = G(I)  .1y + T· 8
l.e. G(II)
_
GS = L.1T
Tm
YLV
m
where .1y =
Ysv 
YSL 
YLV
This is shown in the figure below:
G(I)
/ly
Note that as 8 ~ 0, G(II) ~ G(I), which means that in practice YSL + YLV ~ Ysv as a result of an interaction between the S/L and LlV interfaces as they approach to within atomic dimensions of each other. The optimum liquid layer thickness (8 0 ) will be that giving a minimum free energy as shown. We cannot calculate this value
Solutions to exercises
480
without a knowledge of the above interaction. However, it is reasonable to assurne that the minimum will occur at aseparation of a few atom diameters, provided omax in the above diagram is at least a few atom diameters. omax is defined by G(I) = G(I1) LI1T
i.e. G(I) = G(I)  l1y + T·
omax
m
.
AlternatIvely, I1T =
l1yT
Vm U max
If omax = 10 nm (say), then I1T = 16 K. It seems therefore that surface melting is theoretically possible a few degrees below Tm.
4.11
(a) Repeated surface nucleation (see Section 4.2.2, p. 198).
,
G
r
hl
t
L
s
Suppose the edge of the cap nucleus is associated with an energy e (J rnI). Formation of such a cap will cause a free energy change given by I1G
= nr 2hl1Gv + 2nre
The critical cap radius r* is given by d(I1G) = 0 dr
.
l.e. r
*
e
= hl1G v
and
The rate at WhiC(h_c;~s*)nucleate on the surface should be proportional to exp
~
Solurions to exercises
481
But, t1G oc t1Tj , the undercooling at the interface, so for sm all undercoolings we have N
(k) nuc el m~2 s~l I·
exp 
oc
t1Tj
where k is approximately constant. Each time a cap is nucleated, it should grow rapidly across the interface to advance a distance h. It seems reasonable to suppose therefore that the growth rate will be proportional to N, i.e. v
oc
k
expt1Tj
(b) Very roughly, Equation 4.28 can be seen to be reasonable as folIows: Firstly, it is reasonable to suppose that the distance between successive turns of the spiral (L) will be linearly related to the minimum radius at the centre (r*). Thus we have L oc r* oc t1Ti l
Secondly, for sm all undercoolings, the lateral velocity of the steps (u) should be proportional to the driving force, which in turn is proportional to t1 Tj u
oc
t1Tj
Thus the velocity normal to the interface v is given by uh v = L
oc
t1T2 I
where h is the step height. 4.12
Equilibrium solidification (see Figs. 4.19 and 4.20)
From Fig. 4.19 the lever rule gives the mole fraction solid (fs) at T2 as
fs
Xs
= XL
 Xo = (Xs/k)  Xo XL  X s (Xs/k)  X s
=
kXo 1(1'k)f:s
482
Solutions to exercises
This expression relates the composition of the solid forming at the interface at T2 to the fraction already solidified. For the case shown in Fig. 4.19, it will be roughly as shown below:
t
x.
o
f.
The temperature of the interface (T2 ) as a function of the fraction solidified can be obtained using the following relationship which is apparent from Fig. 4.19 T2  T3 Xo  X s = Tl  T3 X o  kXo
Substituting for X s gives
~: =~:
= {I
+k
C~ fs) fl
This will be a curved line roughly as shown below for the case described for Fig. 4.19 (k  0.47).
T3 +~.
o
Solutions to exercises
483
No diffusion in solid, perfect mixing in liquid (see Fig. 4.21).
Again, we have Xo  Xs X o  kXo
T2  T3 Tl  T3
X s is now given by Equation 4.33 such that T2

X o  kXo(1  fs)(kl) X o  kXo
T3
1  k(l  fs)(kl) (1  k) where Tl > T2 > TE' For the phase diagram in Fig. 4.21a, the following variation is therefore obtained (k  0.47, the exact form of the curve depends on k, of course)
o
f.
No diffusion in solid, no stirring in liquid (see Fig. 4.22)
T,
t
Initial transient Sieady state
~+
o
Final transient
____________________L _ _ _ __ _ f.
Solutions to exercises
484
4.13 No diffusion in solid, complete mixing in liquid
s
Xo
x
kXo
(b)
kXo
o+~=~~
o

So/utions to exercises
485
Diagram (a), above, is a typical phase diagram for k > 1. (In this case, k = 3.) The variation of composition along the bar can be calculated using Equation 4.33 i.e. X s = kXo(l  fs)(kl) The result for k = 3 is shown in diagram (b). fs is proportional to distance along the bar. Note that the final composition to solidify is pure solvent (Xs = 0). No diffusion in solid, no stirring in liquid. kXo
Steady state
Xo
o+~~~
o
4.14
During steadystate growth the concentration profile in the liquid must be such that the rate at which solute diffuses down the concentration gradient away from the interface is balanced by the rate at which solute is rejected from the solidifying liquid, i.e. DC{ = v(CL

Cs)
Assuming the molar volume is independent of composition, this becomes
~~XL = V (~o

X o) at the interface
The concentration profile in the liquid is given by XL =
X{l  1 ~ k. exp  (D~V)} O
~L = XoC ~ k).; ·exp v
= (Xo  Xd D
(;;V)
Solutions to exercises
486
Substituting this expression into the solute equation
v (Xo  Xd = v D· D
(Xko  X o)
Since XL = Xo/k at the interface, the expressions are equivalent, and the profile satisfies the solute balance. 4.15 700
5004~rr~~~~r~
o
5
15
10
25
20
30
35 Xsolute
For an AIO.5 wt% Cu alloy:
(a) Interface temperature in the steady state is given by the sol idus temperature for the composition concerned, Interface temperature
=
650.1°e
(b) Diffusion layer thickness is equivalent to the characteristic width of the concentration profile, .
DL
Thlckness = 
v
=
3 X 10 9 =6 5 x 10 6
X
10 4 m
(c) A plan ar interface is only stable if there is no zone of constituti on al undercooling ahead of it. Under steadystate growth, consideration of the temperature and concentration profiles in the liquid ah"ead of the interface gives that the critical gradient, TL, can be expressed as follows T'  Tl  T3 L D/v
Th
us
where Tl = liquidus temp at X o T3 = solidus temp at X o
T'  (658.3  650.1) oe I L 6 X 104 m
= 13.7 K mm I
487
Solutions to exercises
(d) For an AI2 wt% Cu altoy: Interface temperature
4.16
= 620.4°C
.. . DIffusIOn layer thickness
= 5 x 10 6 = 6
. Temperature gradIent
(653.2  620.4) 6 X 10 4
Scheil equation: XL
=
3
X
10 9
X
10 4 m
= 54.7 K mm 1
= xo/Lkl)
Since it is assumed that the solidus and liquidus lines are straight, k is constant over the solidification range, and may be calculated using X max and XE as follows Xs . k = XL at a gIven temperature
At the eutectic temperature, X s Thus, k
= X max and XL = XE'
5.65
= 33.0 = 0.17
33
5.65 ~o
~
0.341========================.,1 kXo o
0.88 0.97
Distance along bar
The above plot may be constructed by considering the composition of the initial solid formed (kXo), the position at which the solid has the compositions X o and X max , and the eutectic composition, XE' Initial solid formed = kXo.
= 0.17 x 2 wt% Cu = 0.34 wt% Cu
Solutions to exercises
488
The volume fraction of liquid remaining, A when the solid deposited has a composition X o is found from the Scheil equation. Thus when X s
= X o; XL = ~O,
and the Scheit equation becomes
X o = X. f(kl) k 0 L
_1_ 0.17
= f( 0.83) L
A = 0.12, hence fs (position along bar) = 0.88 Simitarly, when X s becomes 5.65 0.17
=2
x
=
X max
=
5.65wt% Cu, the Scheit equation
f(0.83) L
_ (0.17 X 5.65
A
2)110.83
= 0.03 Hence fs (position along bar) = 0.97 From the information given, XE = 33 wt% Cu for positions along the bar between 0.97 and 1. (b) From the diagram, the fraction solidifying as a eutectic, JE = 0.03. (c) For an AI0.5 wt% Cu alloy solidified under the same conditions, the fraction forming as eutectic may be found from the Scheil equation as before by putting X s equal to X max : f(kl) X L X. 0 L X s _ X. f(kl) k 0 L
X max _ X. f(kl) k  0 L
5.65 0.17
= 05 .
x
f(0.83) E
_ (0.17 X 0.5)110.83 5.65
fE 
= 0.006
489
Solutions to exercises
4.17
Cells grow in the direction of maximum temperature gradient, which is upstream in a convection current.
4.18
L
T,
d
h
I
y
I
I
0.25
Assurne equilibrium conditions between J and L
L
t
Temperalure al which all /) disappeared
4.19
It can be shown that the growth rate of a lamellar eutectic v, is given by the following equation
v
*)
1 ( 1  A = kDI1.T.o . A A
where k = D = I1.To = A= A* =
proportionality constant; liquid diffusivity; interface undercooling; lamellar spacing; minimum possible value of A.
490
Solutions to exercises (i) When the undercooling is fixed, k, D and I1To may be combined to form a constant c, thus
v=C.~.(l~*) Differentiating this equation with respect to A dv dA
c
2CA*
=)1+Y
·ff .. d· d 2v 2c Dl erentIatmg a secon time: dA 2 = A3

6CA * y.
C 2CA * . Hence A2 = Y at the max. or mm. growth rate. A = 2A* Substituting this value into the equation of the second differential d 2v dA 2
=
2c A3
6CA*

Y
2c 6CA *  8A *3  16A *4 C
 8A *3 Thus when A = 2A *, the growth rate is a maximum.
(ii) When the growth rate is fixed, the original equation may be rewritten as follows
*)
A a=I1To ·i1 ( IT where
v a=kD
a
Thus: I1To =
1
i 
A* A2
Differentiating with respect to A
a dl1To 1 2A * I1 T6· ~ =  A2 + A3 dl1To _ I1T6 ( 1  ; A2
~

2A
*)
):}
Solutions to exercises
491
Differentiating a second time
a d2~To
d~To
2a
2
61. *
~Tr dA2 + ~·~TÖ = 1.3  1.4 a d2 ßTo
2 (1
21.*)
~To· dA2 + ~To 1.2  1.3
=
(2 61.*) 1.3  1.4
d2~TÖ = 2~To (~ _ 21.*) _ ßTÖ (~ _ 61.*) dA2
1.2
a
Substituting I.
d2~To
1.3
a
1.3
1.4
= 21.*
2~To ( 1 1) ~TÖ ( 1 6) = a 41.*2  41.*2  ;; 41.*3  161.*3
dA2
.. Thus d2~To. dA 2 IS posItIve Hence undercooling is a minimum when A. 4.20
= 2A *
The total change in molar free energy when liquid transforms into lamella a + ß with a spacing I. is given by Equation 4.37, i.e.
~G(A) = ~G(oo) + 2YaßVrn I.
The equilibrium eutectic temperature TE is defined by A. = 00 and G(oo) = O. We can define a metastable equilibrium eutectic temperature at (TE  ~TE) such that at this temperature there is no change in free energy when L ~ a + ß with a spacing A, i.e. at TE  ßTE , ßG(A) = o. Also from Equation 4.38 at an undercooling of ~TE
~G(oo) = ~H~TE TE
Finally, then, combining these equations gives
~TE
= 2YaßVrn TE ~
Substituting: Yaß gives ~TE
10 6
=
I.
i.e. for A = 0.2
I.
=
~H
= 0.4 J m 2, TE = 1000 K, Vrn = 8
ßTE = 5 K 1.0 11m, ~TE = 1 K ~m,
X
108 J m 3
Solutions to exercises
492
Note that if these eutectics grow at the optimum spacing of 21..* the total undercooling at the interface during growth (ATo) will be given by Equation 4.39 such that for I.. and I..
= 0.2 11m, 1..* = 0.1 11m, = 1.0 11m, 1..* = 0.5 11m,
= 10 K ATo = 2 K ATo
4.21
ß
a
ß
ß
a
1,,1
I,,j
Lamellar eutectic
Rodlike euleclic
For a lamellar eutectic the total interfacial area per unit volume of eutectic is given by: 2/1.., irrespective of volume fraction of ß. For the rod eutectic, considering rods of unit length, and diameter d, the area of a/ß interface per unit volume of eutectic is given by
nd 2nd A' A{312 = 1..2
13
For the rod eutectic to have the minimum interfacial energy, then
2nd 2 A2 {3
View more...
Comments